#------------------------------------------------------------------------------
#$Date: 2016-03-02 07:24:58 +0200 (Wed, 02 Mar 2016) $
#$Revision: 177118 $
#$URL: svn://www.crystallography.net/cod/cif/7/03/86/7038647.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7038647
loop_
_publ_author_name
'Kim, Yonghwi'
'Haldar, Ritesh'
'Kim, Hyunuk'
'Koo, Jaehyoung'
'Kim, Kimoon'
_publ_section_title
;
 The guest-dependent thermal response of the flexible MOF
 Zn2(BDC)2(DABCO).
;
_journal_issue                   10
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              4187
_journal_page_last               4192
_journal_paper_doi               10.1039/c5dt03710g
_journal_volume                  45
_journal_year                    2016
_chemical_formula_sum            'C22 H20 N2 O8 Zn2'
_chemical_formula_weight         571.14
_chemical_name_common            '[Zn2(BDC)2(DABCO)]'
_chemical_name_systematic
; 
 ? 
;
_space_group_crystal_system      tetragonal
_space_group_IT_number           123
_space_group_name_Hall           '-P 4 2'
_space_group_name_H-M_alt        'P 4/m m m'
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014
_audit_update_record
;
2015-10-14 deposited with the CCDC.
2015-10-15 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   10.9504(3)
_cell_length_b                   10.9504(3)
_cell_length_c                   9.6032(3)
_cell_measurement_reflns_used    5402
_cell_measurement_temperature    200(2)
_cell_measurement_theta_max      46.87
_cell_measurement_theta_min      2.63
_cell_volume                     1151.53(6)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-97 (Sheldrick 2008)'
_diffrn_ambient_temperature      200(2)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.962
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0289
_diffrn_reflns_av_unetI/netI     0.0225
_diffrn_reflns_laue_measured_fraction_full 0.993
_diffrn_reflns_laue_measured_fraction_max 0.962
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            7758
_diffrn_reflns_point_group_measured_fraction_full 0.993
_diffrn_reflns_point_group_measured_fraction_max 0.962
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         33.137
_diffrn_reflns_theta_min         2.630
_exptl_absorpt_coefficient_mu    1.067
_exptl_absorpt_correction_T_max  0.7494
_exptl_absorpt_correction_T_min  0.5320
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    0.824
_exptl_crystal_description       block
_exptl_crystal_F_000             290
_exptl_crystal_size_max          0.250
_exptl_crystal_size_mid          0.240
_exptl_crystal_size_min          0.200
_refine_diff_density_max         0.959
_refine_diff_density_min         -0.666
_refine_diff_density_rms         0.065
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.072
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     39
_refine_ls_number_reflns         1280
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.072
_refine_ls_R_factor_all          0.0328
_refine_ls_R_factor_gt           0.0286
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0255P)²+0.5253P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0626
_refine_ls_wR_factor_ref         0.0648
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1190
_reflns_number_total             1280
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c5dt03710g2.cif
_cod_data_source_block           DMOF-200K
_cod_original_cell_volume        1151.53(7)
_cod_database_code               7038647
_shelx_space_group_comment
; 
The symmetry employed for this shelxl refinement is uniquely defined 
by the following loop, which should always be used as a source of 
symmetry information in preference to the above space-group names. 
They are only intended as comments. 
;
_shelx_estimated_absorpt_t_min   0.776
_shelx_estimated_absorpt_t_max   0.815
_shelxl_version_number           2014-3
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-y, x, z'
'y, -x, z'
'-x, y, -z'
'x, -y, -z'
'y, x, -z'
'-y, -x, -z'
'-x, -y, -z'
'x, y, -z'
'y, -x, -z'
'-y, x, -z'
'x, -y, z'
'-x, y, z'
'-y, -x, z'
'y, x, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Zn1 Zn 0.0000 1.0000 0.34998(3) 0.01143(9) Uani 1 8 d S T P
O1 O 0.18270(12) 1.0163(5) 0.38467(14) 0.0228(9) Uani 0.5 1 d . . P
N1 N 0.0000 1.0000 0.1341(2) 0.0143(4) Uani 1 8 d S T P
C1 C 0.23529(17) 1.0000 0.5000 0.0215(4) Uani 1 4 d S T P
C2 C 0.37258(17) 1.0000 0.5000 0.0238(4) Uani 1 4 d S T P
C3 C 0.43666(15) 1.0000 0.62239(17) 0.0550(7) Uani 1 2 d S T P
H3 H 0.3938 1.0000 0.7084 0.066 Uiso 1 2 calc R U P
C4 C 0.0478(5) 1.1136(3) 0.0799(3) 0.069(3) Uani 0.375 1 d . . P
H4A H 0.1322 1.1256 0.1142 0.083 Uiso 0.75 2 calc R U P
H4B H -0.0027 1.1824 0.1142 0.083 Uiso 0.75 2 calc R U P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Zn1 O1 78.5(3) . 16_465
O1 Zn1 O1 10.0(3) . 13_575
O1 Zn1 O1 88.466(13) 16_465 13_575
O1 Zn1 O1 88.466(13) . 3_665
O1 Zn1 O1 10.0(3) 16_465 3_665
O1 Zn1 O1 98.4(3) 13_575 3_665
O1 Zn1 O1 98.4(3) . 15_665
O1 Zn1 O1 161.16(8) 16_465 15_665
O1 Zn1 O1 88.466(13) 13_575 15_665
O1 Zn1 O1 158.61(15) 3_665 15_665
O1 Zn1 O1 161.16(8) . 2_575
O1 Zn1 O1 98.4(3) 16_465 2_575
O1 Zn1 O1 158.61(15) 13_575 2_575
O1 Zn1 O1 88.466(13) 3_665 2_575
O1 Zn1 O1 78.5(3) 15_665 2_575
O1 Zn1 O1 158.61(15) . 14
O1 Zn1 O1 88.466(13) 16_465 14
O1 Zn1 O1 161.16(8) 13_575 14
O1 Zn1 O1 78.5(3) 3_665 14
O1 Zn1 O1 88.466(13) 15_665 14
O1 Zn1 O1 10.0(3) 2_575 14
O1 Zn1 O1 88.465(13) . 4_465
O1 Zn1 O1 158.61(15) 16_465 4_465
O1 Zn1 O1 78.5(3) 13_575 4_465
O1 Zn1 O1 161.16(8) 3_665 4_465
O1 Zn1 O1 10.0(3) 15_665 4_465
O1 Zn1 O1 88.466(13) 2_575 4_465
O1 Zn1 O1 98.4(3) 14 4_465
O1 Zn1 N1 99.42(4) . .
O1 Zn1 N1 99.42(4) 16_465 .
O1 Zn1 N1 99.42(4) 13_575 .
O1 Zn1 N1 99.42(4) 3_665 .
O1 Zn1 N1 99.42(4) 15_665 .
O1 Zn1 N1 99.42(4) 2_575 .
O1 Zn1 N1 99.42(4) 14 .
O1 Zn1 N1 99.42(4) 4_465 .
O1 Zn1 Zn1 80.58(4) . 9_576
O1 Zn1 Zn1 80.58(4) 16_465 9_576
O1 Zn1 Zn1 80.58(4) 13_575 9_576
O1 Zn1 Zn1 80.58(4) 3_665 9_576
O1 Zn1 Zn1 80.58(4) 15_665 9_576
O1 Zn1 Zn1 80.58(4) 2_575 9_576
O1 Zn1 Zn1 80.58(4) 14 9_576
O1 Zn1 Zn1 80.58(4) 4_465 9_576
N1 Zn1 Zn1 180.0 . 9_576
O1 O1 C1 81.9(2) 13_575 .
O1 O1 Zn1 84.98(14) 13_575 .
C1 O1 Zn1 125.46(14) . .
C4 N1 C4 41.3(4) 16_465 .
C4 N1 C4 118.6(4) 16_465 3_665
C4 N1 C4 82.56(9) . 3_665
C4 N1 C4 82.56(9) 16_465 14
C4 N1 C4 42.4(4) . 14
C4 N1 C4 41.3(4) 3_665 14
C4 N1 C4 42.4(4) 16_465 4_465
C4 N1 C4 82.56(9) . 4_465
C4 N1 C4 137.8(3) 3_665 4_465
C4 N1 C4 119.5(4) 14 4_465
C4 N1 C4 137.8(3) 16_465 15_665
C4 N1 C4 119.5(4) . 15_665
C4 N1 C4 42.4(4) 3_665 15_665
C4 N1 C4 82.56(9) 14 15_665
C4 N1 C4 118.6(4) 4_465 15_665
C4 N1 C4 119.5(4) 16_465 2_575
C4 N1 C4 137.8(3) . 2_575
C4 N1 C4 82.56(9) 3_665 2_575
C4 N1 C4 118.6(4) 14 2_575
C4 N1 C4 82.56(9) 4_465 2_575
C4 N1 C4 41.3(4) 15_665 2_575
C4 N1 C4 82.56(9) 16_465 13_575
C4 N1 C4 118.6(4) . 13_575
C4 N1 C4 119.5(4) 3_665 13_575
C4 N1 C4 137.8(3) 14 13_575
C4 N1 C4 41.3(4) 4_465 13_575
C4 N1 C4 82.56(9) 15_665 13_575
C4 N1 C4 42.4(4) 2_575 13_575
C4 N1 Zn1 111.09(14) 16_465 .
C4 N1 Zn1 111.09(14) . .
C4 N1 Zn1 111.09(14) 3_665 .
C4 N1 Zn1 111.09(14) 14 .
C4 N1 Zn1 111.09(14) 4_465 .
C4 N1 Zn1 111.09(14) 15_665 .
C4 N1 Zn1 111.09(14) 2_575 .
C4 N1 Zn1 111.09(14) 13_575 .
O1 C1 O1 125.7(2) 13_575 10_556
O1 C1 O1 122.9(2) 13_575 6_576
O1 C1 O1 16.3(4) 10_556 6_576
O1 C1 O1 16.3(4) 13_575 .
O1 C1 O1 122.9(2) 10_556 .
O1 C1 O1 125.7(2) 6_576 .
O1 C1 C2 117.17(10) 13_575 .
O1 C1 C2 117.17(10) 10_556 .
O1 C1 C2 117.17(10) 6_576 .
O1 C1 C2 117.17(10) . .
C3 C2 C3 118.33(19) 10_556 .
C3 C2 C1 120.84(10) 10_556 .
C3 C2 C1 120.84(10) . .
C2 C3 C3 120.84(10) . 2_675
N1 C4 C4 111.09(14) . 10
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Zn1 O1 2.0361(14) .
Zn1 O1 2.0361(13) 16_465
Zn1 O1 2.0361(14) 13_575
Zn1 O1 2.0361(13) 3_665
Zn1 O1 2.0361(13) 15_665
Zn1 O1 2.0361(14) 2_575
Zn1 O1 2.0361(14) 14
Zn1 O1 2.0361(13) 4_465
Zn1 N1 2.073(2) .
Zn1 Zn1 2.8814(6) 9_576
O1 O1 0.357(10) 13_575
O1 C1 1.2609(17) .
N1 C4 1.447(3) 16_465
N1 C4 1.447(3) .
N1 C4 1.447(3) 3_665
N1 C4 1.447(3) 14
N1 C4 1.447(3) 4_465
N1 C4 1.447(3) 15_665
N1 C4 1.447(3) 2_575
N1 C4 1.447(3) 13_575
C1 O1 1.2609(17) 13_575
C1 O1 1.2609(17) 10_556
C1 O1 1.2609(17) 6_576
C1 C2 1.503(3) .
C2 C3 1.3688(19) 10_556
C2 C3 1.3688(19) .
C3 C3 1.387(3) 2_675
C4 C4 1.534(5) 10
